# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2017

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_x
_database_code_depnum_ccdc_archive 'CCDC 1522516'
_audit_update_record             
;
2016-12-13 deposited with the CCDC.
2017-03-21 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'Co O6 Te, 4(Na) '
_chemical_formula_sum            'Co Na4 O6 Te'
_chemical_formula_weight         374.49

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'P 2/c'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'

_cell_length_a                   5.677(5)
_cell_length_b                   9.524(7)
_cell_length_c                   5.485(4)
_cell_angle_alpha                90.00
_cell_angle_beta                 109.470(14)
_cell_angle_gamma                90.00
_cell_volume                     279.6(4)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    854
_cell_measurement_theta_min      2.1384
_cell_measurement_theta_max      27.4662

_exptl_crystal_description       slice
_exptl_crystal_colour            purple
_exptl_crystal_size_max          0.2500
_exptl_crystal_size_mid          0.1800
_exptl_crystal_size_min          0.0500
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    4.448
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             342
_exptl_absorpt_coefficient_mu    8.461
_exptl_absorpt_correction_type   Multi-scan
_exptl_absorpt_correction_T_min  0.6929
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_process_details   ?

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Saturn724+ (2x2 bin mode)'
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_detector_area_resol_mean 28.5714
_diffrn_standards_number         669
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            2033
_diffrn_reflns_av_R_equivalents  0.0393
_diffrn_reflns_av_sigmaI/netI    0.0410
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_theta_min         4.28
_diffrn_reflns_theta_max         27.47
_reflns_number_total             634
_reflns_number_gt                558
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0192P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   none
_refine_ls_hydrogen_treatment    none
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         634
_refine_ls_number_parameters     59
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0243
_refine_ls_R_factor_gt           0.0222
_refine_ls_wR_factor_ref         0.0493
_refine_ls_wR_factor_gt          0.0489
_refine_ls_goodness_of_fit_ref   0.971
_refine_ls_restrained_S_all      0.971
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Te1 Te 0.5000 0.25660(3) 0.7500 0.00566(13) Uani 1 2 d S . .
Co1 Co 0.5000 0.58532(6) 0.7500 0.0077(2) Uani 1 2 d S . .
O1 O 0.2988(5) 0.4093(2) 0.5308(5) 0.0077(6) Uani 1 1 d . . .
O2 O 0.6986(5) 0.2679(2) 0.5231(5) 0.0082(6) Uani 1 1 d . . .
O3 O 0.2816(5) 0.1184(3) 0.5415(5) 0.0082(5) Uani 1 1 d . . .
Na1 Na 0.5000 0.08151(18) 0.2500 0.0050(5) Uani 1 2 d S . .
Na2 Na 0.0000 0.5721(2) 0.2500 0.0115(5) Uani 1 2 d S . .
Na3 Na 0.0000 0.2577(2) 0.2500 0.0179(6) Uani 1 2 d S . .
Na4 Na 0.0000 0.0820(2) 0.7500 0.0189(6) Uani 1 2 d S . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Te1 O3 1.906(3) . ?
Te1 O3 1.906(3) 2_656 ?
Te1 O2 1.941(3) . ?
Te1 O2 1.941(3) 2_656 ?
Te1 O1 1.988(3) 2_656 ?
Te1 O1 1.988(3) . ?
Te1 Na1 3.210(2) . ?
Te1 Na1 3.210(2) 1_556 ?
Te1 Na1 3.220(3) 3_656 ?
Te1 Na3 3.2232(19) 1_656 ?
Te1 Na3 3.2232(19) . ?
Te1 Na2 3.274(2) 3_666 ?
Co1 O2 2.084(3) 4_566 ?
Co1 O2 2.084(3) 3_666 ?
Co1 O1 2.155(3) . ?
Co1 O1 2.155(3) 2_656 ?
Co1 O1 2.203(3) 4_566 ?
Co1 O1 2.203(3) 3_666 ?
Co1 Na1 3.173(3) 3_666 ?
Co1 Na3 3.208(2) 3_666 ?
Co1 Na3 3.208(2) 3_566 ?
Co1 Na2 3.210(2) 3_566 ?
Co1 Na2 3.210(2) 3_666 ?
Co1 Na2 3.2257(19) . ?
O1 Co1 2.203(3) 3_666 ?
O1 Na3 2.365(3) . ?
O1 Na2 2.390(3) 3_566 ?
O1 Na2 2.431(3) . ?
O2 Co1 2.084(3) 3_666 ?
O2 Na2 2.319(3) 3_666 ?
O2 Na1 2.354(3) . ?
O2 Na4 2.489(3) 1_655 ?
O2 Na3 2.625(3) 1_655 ?
O3 Na3 2.273(3) . ?
O3 Na4 2.281(3) . ?
O3 Na1 2.351(3) 3_656 ?
O3 Na1 2.354(3) . ?
O3 Na4 2.655(3) 3_556 ?
Na1 O2 2.354(3) 2_655 ?
Na1 O3 2.351(3) 4 ?
Na1 O3 2.351(3) 3_656 ?
Na1 O3 2.354(3) 2_655 ?
Na1 Na1 3.152(2) 3_655 ?
Na1 Na1 3.152(2) 3_656 ?
Na1 Co1 3.173(3) 3_666 ?
Na1 Te1 3.210(2) 1_554 ?
Na1 Te1 3.220(3) 3_656 ?
Na2 O2 2.319(3) 3_666 ?
Na2 O2 2.319(3) 4_465 ?
Na2 O1 2.390(3) 4_565 ?
Na2 O1 2.390(3) 3_566 ?
Na2 O1 2.431(3) 2 ?
Na2 Na3 2.994(4) . ?
Na2 Na2 3.067(3) 3_565 ?
Na2 Na2 3.067(3) 3_566 ?
Na2 Na3 3.186(2) 3_566 ?
Na2 Na3 3.186(2) 3_565 ?
Na2 Co1 3.210(2) 3_566 ?
Na3 O3 2.273(3) 2 ?
Na3 O1 2.365(3) 2 ?
Na3 O2 2.625(3) 2_655 ?
Na3 O2 2.625(3) 1_455 ?
Na3 Na2 3.186(2) 3_566 ?
Na3 Na2 3.186(2) 3_565 ?
Na3 Co1 3.208(2) 3_666 ?
Na3 Co1 3.208(2) 3_566 ?
Na3 Na4 3.213(2) 1_554 ?
Na4 O3 2.281(3) 2_556 ?
Na4 O2 2.489(3) 2_656 ?
Na4 O2 2.489(3) 1_455 ?
Na4 O3 2.655(3) 3_556 ?
Na4 O3 2.655(3) 4_556 ?
Na4 Na4 3.156(3) 3_556 ?
Na4 Na4 3.156(3) 3_557 ?
Na4 Na3 3.213(2) 1_556 ?
Na4 Na1 3.2232(19) 1_455 ?
Na4 Na1 3.2232(19) 1_556 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3 Te1 O3 92.65(16) . 2_656 ?
O3 Te1 O2 93.12(12) . . ?
O3 Te1 O2 91.28(12) 2_656 . ?
O3 Te1 O2 91.28(12) . 2_656 ?
O3 Te1 O2 93.12(12) 2_656 2_656 ?
O2 Te1 O2 173.62(14) . 2_656 ?
O3 Te1 O1 174.96(9) . 2_656 ?
O3 Te1 O1 90.83(12) 2_656 2_656 ?
O2 Te1 O1 90.44(12) . 2_656 ?
O2 Te1 O1 84.89(12) 2_656 2_656 ?
O3 Te1 O1 90.83(12) . . ?
O3 Te1 O1 174.96(9) 2_656 . ?
O2 Te1 O1 84.89(12) . . ?
O2 Te1 O1 90.44(12) 2_656 . ?
O1 Te1 O1 85.93(15) 2_656 . ?
O3 Te1 Na1 46.67(8) . . ?
O3 Te1 Na1 88.20(9) 2_656 . ?
O2 Te1 Na1 46.81(8) . . ?
O2 Te1 Na1 137.92(8) 2_656 . ?
O1 Te1 Na1 137.17(8) 2_656 . ?
O1 Te1 Na1 91.54(9) . . ?
O3 Te1 Na1 88.20(9) . 1_556 ?
O3 Te1 Na1 46.67(8) 2_656 1_556 ?
O2 Te1 Na1 137.92(8) . 1_556 ?
O2 Te1 Na1 46.81(8) 2_656 1_556 ?
O1 Te1 Na1 91.54(9) 2_656 1_556 ?
O1 Te1 Na1 137.17(8) . 1_556 ?
Na1 Te1 Na1 117.40(7) . 1_556 ?
O3 Te1 Na1 46.33(8) . 3_656 ?
O3 Te1 Na1 46.33(8) 2_656 3_656 ?
O2 Te1 Na1 93.19(7) . 3_656 ?
O2 Te1 Na1 93.19(7) 2_656 3_656 ?
O1 Te1 Na1 137.03(7) 2_656 3_656 ?
O1 Te1 Na1 137.03(7) . 3_656 ?
Na1 Te1 Na1 58.70(4) . 3_656 ?
Na1 Te1 Na1 58.70(4) 1_556 3_656 ?
O3 Te1 Na3 136.48(9) . 1_656 ?
O3 Te1 Na3 43.89(9) 2_656 1_656 ?
O2 Te1 Na3 90.60(10) . 1_656 ?
O2 Te1 Na3 89.38(10) 2_656 1_656 ?
O1 Te1 Na3 46.94(8) 2_656 1_656 ?
O1 Te1 Na3 132.68(8) . 1_656 ?
Na1 Te1 Na3 118.55(5) . 1_656 ?
Na1 Te1 Na3 61.67(5) 1_556 1_656 ?
Na1 Te1 Na3 90.19(4) 3_656 1_656 ?
O3 Te1 Na3 43.89(9) . . ?
O3 Te1 Na3 136.48(9) 2_656 . ?
O2 Te1 Na3 89.38(10) . . ?
O2 Te1 Na3 90.60(10) 2_656 . ?
O1 Te1 Na3 132.68(8) 2_656 . ?
O1 Te1 Na3 46.94(8) . . ?
Na1 Te1 Na3 61.67(5) . . ?
Na1 Te1 Na3 118.55(5) 1_556 . ?
Na1 Te1 Na3 90.19(4) 3_656 . ?
Na3 Te1 Na3 179.63(7) 1_656 . ?
O3 Te1 Na2 137.30(8) . 3_666 ?
O3 Te1 Na2 87.33(10) 2_656 3_666 ?
O2 Te1 Na2 44.23(8) . 3_666 ?
O2 Te1 Na2 131.39(8) 2_656 3_666 ?
O1 Te1 Na2 46.51(8) 2_656 3_666 ?
O1 Te1 Na2 87.64(9) . 3_666 ?
Na1 Te1 Na2 90.69(4) . 3_666 ?
Na1 Te1 Na2 120.39(2) 1_556 3_666 ?
Na1 Te1 Na2 119.89(4) 3_656 3_666 ?
Na3 Te1 Na2 58.72(5) 1_656 3_666 ?
Na3 Te1 Na2 121.06(5) . 3_666 ?
O2 Co1 O2 95.76(14) 4_566 3_666 ?
O2 Co1 O1 169.07(10) 4_566 . ?
O2 Co1 O1 93.52(11) 3_666 . ?
O2 Co1 O1 93.52(11) 4_566 2_656 ?
O2 Co1 O1 169.07(10) 3_666 2_656 ?
O1 Co1 O1 77.89(14) . 2_656 ?
O2 Co1 O1 76.37(12) 4_566 4_566 ?
O2 Co1 O1 101.81(11) 3_666 4_566 ?
O1 Co1 O1 96.09(10) . 4_566 ?
O1 Co1 O1 85.98(11) 2_656 4_566 ?
O2 Co1 O1 101.81(11) 4_566 3_666 ?
O2 Co1 O1 76.37(12) 3_666 3_666 ?
O1 Co1 O1 85.98(11) . 3_666 ?
O1 Co1 O1 96.09(10) 2_656 3_666 ?
O1 Co1 O1 177.34(12) 4_566 3_666 ?
O2 Co1 Na1 47.88(7) 4_566 3_666 ?
O2 Co1 Na1 47.88(7) 3_666 3_666 ?
O1 Co1 Na1 141.05(7) . 3_666 ?
O1 Co1 Na1 141.05(7) 2_656 3_666 ?
O1 Co1 Na1 88.67(6) 4_566 3_666 ?
O1 Co1 Na1 88.67(6) 3_666 3_666 ?
O2 Co1 Na3 54.60(8) 4_566 3_666 ?
O2 Co1 Na3 87.37(9) 3_666 3_666 ?
O1 Co1 Na3 131.83(8) . 3_666 ?
O1 Co1 Na3 93.32(9) 2_656 3_666 ?
O1 Co1 Na3 130.86(7) 4_566 3_666 ?
O1 Co1 Na3 47.48(7) 3_666 3_666 ?
Na1 Co1 Na3 62.22(4) 3_666 3_666 ?
O2 Co1 Na3 87.37(9) 4_566 3_566 ?
O2 Co1 Na3 54.60(8) 3_666 3_566 ?
O1 Co1 Na3 93.32(9) . 3_566 ?
O1 Co1 Na3 131.83(8) 2_656 3_566 ?
O1 Co1 Na3 47.48(7) 4_566 3_566 ?
O1 Co1 Na3 130.86(7) 3_666 3_566 ?
Na1 Co1 Na3 62.22(4) 3_666 3_566 ?
Na3 Co1 Na3 124.45(9) 3_666 3_566 ?
O2 Co1 Na2 125.43(8) 4_566 3_566 ?
O2 Co1 Na2 92.67(9) 3_666 3_566 ?
O1 Co1 Na2 48.13(8) . 3_566 ?
O1 Co1 Na2 86.63(9) 2_656 3_566 ?
O1 Co1 Na2 49.17(7) 4_566 3_566 ?
O1 Co1 Na2 132.49(7) 3_666 3_566 ?
Na1 Co1 Na2 117.84(4) 3_666 3_566 ?
Na3 Co1 Na2 179.94(4) 3_666 3_566 ?
Na3 Co1 Na2 55.61(7) 3_566 3_566 ?
O2 Co1 Na2 92.67(9) 4_566 3_666 ?
O2 Co1 Na2 125.43(8) 3_666 3_666 ?
O1 Co1 Na2 86.63(9) . 3_666 ?
O1 Co1 Na2 48.13(8) 2_656 3_666 ?
O1 Co1 Na2 132.49(7) 4_566 3_666 ?
O1 Co1 Na2 49.17(7) 3_666 3_666 ?
Na1 Co1 Na2 117.84(4) 3_666 3_666 ?
Na3 Co1 Na2 55.61(7) 3_666 3_666 ?
Na3 Co1 Na2 179.94(4) 3_566 3_666 ?
Na2 Co1 Na2 124.33(9) 3_566 3_666 ?
O2 Co1 Na2 138.53(8) 4_566 . ?
O2 Co1 Na2 45.83(8) 3_666 . ?
O1 Co1 Na2 48.90(8) . . ?
O1 Co1 Na2 126.62(8) 2_656 . ?
O1 Co1 Na2 94.64(10) 4_566 . ?
O1 Co1 Na2 85.47(10) 3_666 . ?
Na1 Co1 Na2 92.24(4) 3_666 . ?
Na3 Co1 Na2 123.10(5) 3_666 . ?
Na3 Co1 Na2 59.36(5) 3_566 . ?
Na2 Co1 Na2 56.92(5) 3_566 . ?
Na2 Co1 Na2 120.62(5) 3_666 . ?
Te1 O1 Co1 98.09(12) . . ?
Te1 O1 Co1 96.46(11) . 3_666 ?
Co1 O1 Co1 94.02(11) . 3_666 ?
Te1 O1 Na3 95.16(11) . . ?
Co1 O1 Na3 165.93(13) . . ?
Co1 O1 Na3 89.16(10) 3_666 . ?
Te1 O1 Na2 96.38(11) . 3_566 ?
Co1 O1 Na2 89.69(10) . 3_566 ?
Co1 O1 Na2 166.00(13) 3_666 3_566 ?
Na3 O1 Na2 84.13(10) . 3_566 ?
Te1 O1 Na2 171.41(13) . . ?
Co1 O1 Na2 89.18(10) . . ?
Co1 O1 Na2 87.55(10) 3_666 . ?
Na3 O1 Na2 77.25(11) . . ?
Na2 O1 Na2 79.00(10) 3_566 . ?
Te1 O2 Co1 101.98(13) . 3_666 ?
Te1 O2 Na2 100.07(11) . 3_666 ?
Co1 O2 Na2 94.05(11) 3_666 3_666 ?
Te1 O2 Na1 96.24(11) . . ?
Co1 O2 Na1 91.08(11) 3_666 . ?
Na2 O2 Na1 161.48(13) 3_666 . ?
Te1 O2 Na4 95.12(11) . 1_655 ?
Co1 O2 Na4 162.52(13) 3_666 1_655 ?
Na2 O2 Na4 86.44(11) 3_666 1_655 ?
Na1 O2 Na4 83.41(10) . 1_655 ?
Te1 O2 Na3 172.91(13) . 1_655 ?
Co1 O2 Na3 85.07(10) 3_666 1_655 ?
Na2 O2 Na3 79.98(10) 3_666 1_655 ?
Na1 O2 Na3 82.76(9) . 1_655 ?
Na4 O2 Na3 77.80(9) 1_655 1_655 ?
Te1 O3 Na3 100.56(13) . . ?
Te1 O3 Na4 103.22(12) . . ?
Na3 O3 Na4 89.74(11) . . ?
Te1 O3 Na1 97.77(12) . 3_656 ?
Na3 O3 Na1 161.47(13) . 3_656 ?
Na4 O3 Na1 88.69(10) . 3_656 ?
Te1 O3 Na1 97.23(12) . . ?
Na3 O3 Na1 90.89(10) . . ?
Na4 O3 Na1 159.06(14) . . ?
Na1 O3 Na1 84.12(10) 3_656 . ?
Te1 O3 Na4 176.74(13) . 3_556 ?
Na3 O3 Na4 81.66(10) . 3_556 ?
Na4 O3 Na4 79.10(10) . 3_556 ?
Na1 O3 Na4 79.91(10) 3_656 3_556 ?
Na1 O3 Na4 80.29(9) . 3_556 ?
O2 Na1 O2 82.08(14) . 2_655 ?
O2 Na1 O3 169.61(9) . 4 ?
O2 Na1 O3 103.78(10) 2_655 4 ?
O2 Na1 O3 103.78(10) . 3_656 ?
O2 Na1 O3 169.61(9) 2_655 3_656 ?
O3 Na1 O3 71.81(14) 4 3_656 ?
O2 Na1 O3 72.79(11) . . ?
O2 Na1 O3 94.05(11) 2_655 . ?
O3 Na1 O3 98.01(11) 4 . ?
O3 Na1 O3 95.88(10) 3_656 . ?
O2 Na1 O3 94.05(11) . 2_655 ?
O2 Na1 O3 72.79(11) 2_655 2_655 ?
O3 Na1 O3 95.88(10) 4 2_655 ?
O3 Na1 O3 98.01(11) 3_656 2_655 ?
O3 Na1 O3 162.83(15) . 2_655 ?
O2 Na1 Na1 141.85(8) . 3_655 ?
O2 Na1 Na1 87.52(8) 2_655 3_655 ?
O3 Na1 Na1 47.98(7) 4 3_655 ?
O3 Na1 Na1 82.61(10) 3_656 3_655 ?
O3 Na1 Na1 144.84(9) . 3_655 ?
O3 Na1 Na1 47.90(7) 2_655 3_655 ?
O2 Na1 Na1 87.52(8) . 3_656 ?
O2 Na1 Na1 141.85(8) 2_655 3_656 ?
O3 Na1 Na1 82.61(10) 4 3_656 ?
O3 Na1 Na1 47.98(7) 3_656 3_656 ?
O3 Na1 Na1 47.90(7) . 3_656 ?
O3 Na1 Na1 144.84(9) 2_655 3_656 ?
Na1 Na1 Na1 120.97(12) 3_655 3_656 ?
O2 Na1 Co1 41.04(7) . 3_666 ?
O2 Na1 Co1 41.04(7) 2_655 3_666 ?
O3 Na1 Co1 144.09(7) 4 3_666 ?
O3 Na1 Co1 144.09(7) 3_656 3_666 ?
O3 Na1 Co1 81.42(8) . 3_666 ?
O3 Na1 Co1 81.42(8) 2_655 3_666 ?
Na1 Na1 Co1 119.52(6) 3_655 3_666 ?
Na1 Na1 Co1 119.52(6) 3_656 3_666 ?
O2 Na1 Te1 36.95(7) . . ?
O2 Na1 Te1 90.89(9) 2_655 . ?
O3 Na1 Te1 133.34(7) 4 . ?
O3 Na1 Te1 98.94(7) 3_656 . ?
O3 Na1 Te1 36.09(7) . . ?
O3 Na1 Te1 130.77(9) 2_655 . ?
Na1 Na1 Te1 178.22(8) 3_655 . ?
Na1 Na1 Te1 60.82(6) 3_656 . ?
Co1 Na1 Te1 58.70(4) 3_666 . ?
O2 Na1 Te1 90.89(9) . 1_554 ?
O2 Na1 Te1 36.95(7) 2_655 1_554 ?
O3 Na1 Te1 98.94(7) 4 1_554 ?
O3 Na1 Te1 133.34(7) 3_656 1_554 ?
O3 Na1 Te1 130.77(9) . 1_554 ?
O3 Na1 Te1 36.09(7) 2_655 1_554 ?
Na1 Na1 Te1 60.82(6) 3_655 1_554 ?
Na1 Na1 Te1 178.22(8) 3_656 1_554 ?
Co1 Na1 Te1 58.70(4) 3_666 1_554 ?
Te1 Na1 Te1 117.40(7) . 1_554 ?
O2 Na1 Te1 138.96(7) . 3_656 ?
O2 Na1 Te1 138.96(7) 2_655 3_656 ?
O3 Na1 Te1 35.91(7) 4 3_656 ?
O3 Na1 Te1 35.91(7) 3_656 3_656 ?
O3 Na1 Te1 98.58(8) . 3_656 ?
O3 Na1 Te1 98.58(8) 2_655 3_656 ?
Na1 Na1 Te1 60.48(6) 3_655 3_656 ?
Na1 Na1 Te1 60.48(6) 3_656 3_656 ?
Co1 Na1 Te1 180.0 3_666 3_656 ?
Te1 Na1 Te1 121.30(4) . 3_656 ?
Te1 Na1 Te1 121.30(4) 1_554 3_656 ?
O2 Na2 O2 97.85(15) 3_666 4_465 ?
O2 Na2 O1 72.60(11) 3_666 4_565 ?
O2 Na2 O1 101.63(11) 4_465 4_565 ?
O2 Na2 O1 101.63(11) 3_666 3_566 ?
O2 Na2 O1 72.60(11) 4_465 3_566 ?
O1 Na2 O1 171.49(14) 4_565 3_566 ?
O2 Na2 O1 173.23(9) 3_666 2 ?
O2 Na2 O1 81.07(10) 4_465 2 ?
O1 Na2 O1 101.00(10) 4_565 2 ?
O1 Na2 O1 84.48(11) 3_566 2 ?
O2 Na2 O1 81.07(10) 3_666 . ?
O2 Na2 O1 173.23(9) 4_465 . ?
O1 Na2 O1 84.48(11) 4_565 . ?
O1 Na2 O1 101.00(10) 3_566 . ?
O1 Na2 O1 100.77(14) 2 . ?
O2 Na2 Na3 131.07(7) 3_666 . ?
O2 Na2 Na3 131.07(8) 4_465 . ?
O1 Na2 Na3 94.25(7) 4_565 . ?
O1 Na2 Na3 94.25(7) 3_566 . ?
O1 Na2 Na3 50.39(7) 2 . ?
O1 Na2 Na3 50.39(7) . . ?
O2 Na2 Na2 123.64(8) 3_666 3_565 ?
O2 Na2 Na2 91.96(8) 4_465 3_565 ?
O1 Na2 Na2 51.09(6) 4_565 3_565 ?
O1 Na2 Na2 133.99(8) 3_566 3_565 ?
O1 Na2 Na2 49.92(8) 2 3_565 ?
O1 Na2 Na2 94.20(10) . 3_565 ?
Na3 Na2 Na2 63.41(7) . 3_565 ?
O2 Na2 Na2 91.96(8) 3_666 3_566 ?
O2 Na2 Na2 123.64(8) 4_465 3_566 ?
O1 Na2 Na2 133.99(8) 4_565 3_566 ?
O1 Na2 Na2 51.09(6) 3_566 3_566 ?
O1 Na2 Na2 94.20(10) 2 3_566 ?
O1 Na2 Na2 49.92(8) . 3_566 ?
Na3 Na2 Na2 63.41(7) . 3_566 ?
Na2 Na2 Na2 126.82(14) 3_565 3_566 ?
O2 Na2 Na3 54.23(8) 3_666 3_566 ?
O2 Na2 Na3 85.17(9) 4_465 3_566 ?
O1 Na2 Na3 126.79(8) 4_565 3_566 ?
O1 Na2 Na3 47.59(7) 3_566 3_566 ?
O1 Na2 Na3 132.04(7) 2 3_566 ?
O1 Na2 Na3 88.82(8) . 3_566 ?
Na3 Na2 Na3 120.59(5) . 3_566 ?
Na2 Na2 Na3 176.00(10) 3_565 3_566 ?
Na2 Na2 Na3 57.18(7) 3_566 3_566 ?
O2 Na2 Na3 85.17(9) 3_666 3_565 ?
O2 Na2 Na3 54.23(8) 4_465 3_565 ?
O1 Na2 Na3 47.59(7) 4_565 3_565 ?
O1 Na2 Na3 126.79(8) 3_566 3_565 ?
O1 Na2 Na3 88.82(8) 2 3_565 ?
O1 Na2 Na3 132.04(7) . 3_565 ?
Na3 Na2 Na3 120.59(5) . 3_565 ?
Na2 Na2 Na3 57.18(7) 3_565 3_565 ?
Na2 Na2 Na3 176.00(10) 3_566 3_565 ?
Na3 Na2 Na3 118.82(10) 3_566 3_565 ?
O2 Na2 Co1 143.23(7) 3_666 3_566 ?
O2 Na2 Co1 79.20(9) 4_465 3_566 ?
O1 Na2 Co1 144.13(8) 4_565 3_566 ?
O1 Na2 Co1 42.18(7) 3_566 3_566 ?
O1 Na2 Co1 43.28(7) 2 3_566 ?
O1 Na2 Co1 97.62(10) . 3_566 ?
Na3 Na2 Co1 62.16(4) . 3_566 ?
Na2 Na2 Co1 93.13(6) 3_565 3_566 ?
Na2 Na2 Co1 61.80(4) 3_566 3_566 ?
Na3 Na2 Co1 89.08(3) 3_566 3_566 ?
Na3 Na2 Co1 119.43(2) 3_565 3_566 ?
O3 Na3 O3 108.59(16) 2 . ?
O3 Na3 O1 176.32(8) 2 . ?
O3 Na3 O1 73.43(11) . . ?
O3 Na3 O1 73.43(11) 2 2 ?
O3 Na3 O1 176.32(8) . 2 ?
O1 Na3 O1 104.73(15) . 2 ?
O3 Na3 O2 93.42(10) 2 2_655 ?
O3 Na3 O2 89.07(10) . 2_655 ?
O1 Na3 O2 83.48(10) . 2_655 ?
O1 Na3 O2 93.91(11) 2 2_655 ?
O3 Na3 O2 89.07(10) 2 1_455 ?
O3 Na3 O2 93.42(10) . 1_455 ?
O1 Na3 O2 93.91(11) . 1_455 ?
O1 Na3 O2 83.48(10) 2 1_455 ?
O2 Na3 O2 175.75(13) 2_655 1_455 ?
O3 Na3 Na2 125.71(8) 2 . ?
O3 Na3 Na2 125.71(8) . . ?
O1 Na3 Na2 52.36(7) . . ?
O1 Na3 Na2 52.36(7) 2 . ?
O2 Na3 Na2 87.87(7) 2_655 . ?
O2 Na3 Na2 87.87(7) 1_455 . ?
O3 Na3 Na2 134.48(7) 2 3_566 ?
O3 Na3 Na2 83.88(8) . 3_566 ?
O1 Na3 Na2 48.27(7) . 3_566 ?
O1 Na3 Na2 92.52(9) 2 3_566 ?
O2 Na3 Na2 131.25(8) 2_655 3_566 ?
O2 Na3 Na2 45.80(6) 1_455 3_566 ?
Na2 Na3 Na2 59.41(5) . 3_566 ?
O3 Na3 Na2 83.88(8) 2 3_565 ?
O3 Na3 Na2 134.48(7) . 3_565 ?
O1 Na3 Na2 92.52(9) . 3_565 ?
O1 Na3 Na2 48.27(7) 2 3_565 ?
O2 Na3 Na2 45.80(6) 2_655 3_565 ?
O2 Na3 Na2 131.25(8) 1_455 3_565 ?
Na2 Na3 Na2 59.41(5) . 3_565 ?
Na2 Na3 Na2 118.82(10) 3_566 3_565 ?
O3 Na3 Co1 133.37(7) 2 3_666 ?
O3 Na3 Co1 81.80(8) . 3_666 ?
O1 Na3 Co1 43.36(7) . 3_666 ?
O1 Na3 Co1 99.09(10) 2 3_666 ?
O2 Na3 Co1 40.33(6) 2_655 3_666 ?
O2 Na3 Co1 136.70(8) 1_455 3_666 ?
Na2 Na3 Co1 62.22(4) . 3_666 ?
Na2 Na3 Co1 90.96(5) 3_566 3_666 ?
Na2 Na3 Co1 60.59(3) 3_565 3_666 ?
O3 Na3 Co1 81.80(8) 2 3_566 ?
O3 Na3 Co1 133.37(7) . 3_566 ?
O1 Na3 Co1 99.09(10) . 3_566 ?
O1 Na3 Co1 43.36(7) 2 3_566 ?
O2 Na3 Co1 136.70(8) 2_655 3_566 ?
O2 Na3 Co1 40.33(6) 1_455 3_566 ?
Na2 Na3 Co1 62.22(4) . 3_566 ?
Na2 Na3 Co1 60.59(3) 3_566 3_566 ?
Na2 Na3 Co1 90.96(5) 3_565 3_566 ?
Co1 Na3 Co1 124.45(9) 3_666 3_566 ?
O3 Na3 Na4 45.23(7) 2 1_554 ?
O3 Na3 Na4 95.53(9) . 1_554 ?
O1 Na3 Na4 132.06(7) . 1_554 ?
O1 Na3 Na4 88.06(8) 2 1_554 ?
O2 Na3 Na4 49.21(6) 2_655 1_554 ?
O2 Na3 Na4 133.79(8) 1_455 1_554 ?
Na2 Na3 Na4 121.39(5) . 1_554 ?
Na2 Na3 Na4 179.20(7) 3_566 1_554 ?
Na2 Na3 Na4 61.98(7) 3_565 1_554 ?
Co1 Na3 Na4 89.48(3) 3_666 1_554 ?
Co1 Na3 Na4 119.64(2) 3_566 1_554 ?
O3 Na4 O3 162.51(17) . 2_556 ?
O3 Na4 O2 70.28(11) . 2_656 ?
O3 Na4 O2 96.95(11) 2_556 2_656 ?
O3 Na4 O2 96.95(11) . 1_455 ?
O3 Na4 O2 70.28(11) 2_556 1_455 ?
O2 Na4 O2 89.27(14) 2_656 1_455 ?
O3 Na4 O3 100.90(10) . 3_556 ?
O3 Na4 O3 91.68(11) 2_556 3_556 ?
O2 Na4 O3 171.19(8) 2_656 3_556 ?
O2 Na4 O3 91.99(10) 1_455 3_556 ?
O3 Na4 O3 91.68(11) . 4_556 ?
O3 Na4 O3 100.90(10) 2_556 4_556 ?
O2 Na4 O3 91.99(10) 2_656 4_556 ?
O2 Na4 O3 171.19(8) 1_455 4_556 ?
O3 Na4 O3 88.09(13) 3_556 4_556 ?
O3 Na4 Na4 55.70(7) . 3_556 ?
O3 Na4 Na4 135.56(8) 2_556 3_556 ?
O2 Na4 Na4 125.99(8) 2_656 3_556 ?
O2 Na4 Na4 96.70(8) 1_455 3_556 ?
O3 Na4 Na4 45.20(7) 3_556 3_556 ?
O3 Na4 Na4 89.61(10) 4_556 3_556 ?
O3 Na4 Na4 135.56(8) . 3_557 ?
O3 Na4 Na4 55.70(7) 2_556 3_557 ?
O2 Na4 Na4 96.70(8) 2_656 3_557 ?
O2 Na4 Na4 125.99(8) 1_455 3_557 ?
O3 Na4 Na4 89.61(10) 3_556 3_557 ?
O3 Na4 Na4 45.20(7) 4_556 3_557 ?
Na4 Na4 Na4 120.67(14) 3_556 3_557 ?
O3 Na4 Na3 123.25(9) . 1_556 ?
O3 Na4 Na3 45.04(7) 2_556 1_556 ?
O2 Na4 Na3 52.99(7) 2_656 1_556 ?
O2 Na4 Na3 81.99(9) 1_455 1_556 ?
O3 Na4 Na3 135.82(6) 3_556 1_556 ?
O3 Na4 Na3 91.81(8) 4_556 1_556 ?
Na4 Na4 Na3 178.27(10) 3_556 1_556 ?
Na4 Na4 Na3 61.05(7) 3_557 1_556 ?
O3 Na4 Na3 45.04(7) . . ?
O3 Na4 Na3 123.25(9) 2_556 . ?
O2 Na4 Na3 81.99(9) 2_656 . ?
O2 Na4 Na3 52.99(7) 1_455 . ?
O3 Na4 Na3 91.81(8) 3_556 . ?
O3 Na4 Na3 135.82(7) 4_556 . ?
Na4 Na4 Na3 61.05(7) 3_556 . ?
Na4 Na4 Na3 178.27(10) 3_557 . ?
Na3 Na4 Na3 117.22(10) 1_556 . ?
O3 Na4 Na1 98.00(9) . 1_455 ?
O3 Na4 Na1 82.03(9) 2_556 1_455 ?
O2 Na4 Na1 133.65(10) 2_656 1_455 ?
O2 Na4 Na1 46.51(7) 1_455 1_455 ?
O3 Na4 Na1 45.89(7) 3_556 1_455 ?
O3 Na4 Na1 133.94(10) 4_556 1_455 ?
Na4 Na4 Na1 60.99(5) 3_556 1_455 ?
Na4 Na4 Na1 118.92(6) 3_557 1_455 ?
Na3 Na4 Na1 118.46(6) 1_556 1_455 ?
Na3 Na4 Na1 61.64(5) . 1_455 ?
O3 Na4 Na1 82.03(9) . 1_556 ?
O3 Na4 Na1 98.00(9) 2_556 1_556 ?
O2 Na4 Na1 46.51(7) 2_656 1_556 ?
O2 Na4 Na1 133.65(10) 1_455 1_556 ?
O3 Na4 Na1 133.94(9) 3_556 1_556 ?
O3 Na4 Na1 45.89(7) 4_556 1_556 ?
Na4 Na4 Na1 118.92(6) 3_556 1_556 ?
Na4 Na4 Na1 60.99(5) 3_557 1_556 ?
Na3 Na4 Na1 61.64(5) 1_556 1_556 ?
Na3 Na4 Na1 118.46(6) . 1_556 ?
Na1 Na4 Na1 179.83(9) 1_455 1_556 ?

_diffrn_measured_fraction_theta_max 0.980
_diffrn_reflns_theta_full        27.47
_diffrn_measured_fraction_theta_full 0.980
_refine_diff_density_max         0.702
_refine_diff_density_min         -0.916
_refine_diff_density_rms         0.200
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_x
_database_code_depnum_ccdc_archive 'CCDC 1522517'
_audit_update_record             
;
2016-12-13 deposited with the CCDC.
2017-03-21 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'Ni O6 Te, 4(Na)'
_chemical_formula_sum            'Na4 Ni O6 Te'
_chemical_formula_weight         374.27

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   'P -1'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   5.405(2)
_cell_length_b                   5.668(2)
_cell_length_c                   9.565(5)
_cell_angle_alpha                73.026(8)
_cell_angle_beta                 89.644(17)
_cell_angle_gamma                80.439(12)
_cell_volume                     276.1(2)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    870
_cell_measurement_theta_min      2.2286
_cell_measurement_theta_max      27.5166

_exptl_crystal_description       Prism
_exptl_crystal_colour            Green
_exptl_crystal_size_max          0.2000
_exptl_crystal_size_mid          0.1500
_exptl_crystal_size_min          0.1000
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    4.502
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             344
_exptl_absorpt_coefficient_mu    8.975
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.8796
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_process_details   ?

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Mercury70 (2x2 bin mode)'
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_detector_area_resol_mean 14.6306
_diffrn_standards_number         1238
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            3493
_diffrn_reflns_av_R_equivalents  0.0148
_diffrn_reflns_av_sigmaI/netI    0.0159
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_theta_min         2.23
_diffrn_reflns_theta_max         27.50
_reflns_number_total             1237
_reflns_number_gt                1190
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0162P)²+0.0965P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   none
_refine_ls_hydrogen_treatment    none
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         1237
_refine_ls_number_parameters     112
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0140
_refine_ls_R_factor_gt           0.0131
_refine_ls_wR_factor_ref         0.0330
_refine_ls_wR_factor_gt          0.0326
_refine_ls_goodness_of_fit_ref   1.152
_refine_ls_restrained_S_all      1.152
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Te1 Te 0.24809(2) 0.99266(2) 0.243136(13) 0.00322(6) Uani 1 1 d . . .
Ni1 Ni 0.25031(5) 1.00294(4) -0.08264(3) 0.00540(8) Uani 1 1 d . . .
O1 O -0.0861(3) 1.1981(3) 0.19870(16) 0.0059(3) Uani 1 1 d . . .
O2 O 0.3473(3) 1.2087(3) 0.34255(16) 0.0067(3) Uani 1 1 d . . .
O3 O 0.5813(3) 0.7872(3) 0.26676(16) 0.0064(3) Uani 1 1 d . . .
O4 O 0.3727(3) 1.1937(3) 0.05633(16) 0.0056(3) Uani 1 1 d . . .
O5 O 0.1259(3) 0.8029(3) 0.12140(16) 0.0056(3) Uani 1 1 d . . .
O6 O 0.1461(3) 0.7745(3) 0.41826(16) 0.0068(3) Uani 1 1 d . . .
Na1 Na 0.0000 0.5000 0.0000 0.0110(3) Uani 1 2 d S . .
Na2 Na 0.50699(16) 0.49297(15) 0.15699(9) 0.0095(2) Uani 1 1 d . . .
Na3 Na 0.98058(17) 0.49337(15) 0.33071(9) 0.0112(2) Uani 1 1 d . . .
Na4 Na 0.5000 0.5000 0.5000 0.0243(4) Uani 1 2 d S . .
Na5 Na 0.25182(14) 0.00391(14) 0.58026(8) 0.0064(2) Uani 1 1 d . . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Te1 O2 1.8962(15) . ?
Te1 O6 1.9089(16) . ?
Te1 O3 1.9506(16) . ?
Te1 O1 1.9550(16) . ?
Te1 O5 1.9813(16) . ?
Te1 O4 1.9991(16) . ?
Te1 Ni1 3.0995(17) . ?
Te1 Ni1 3.1017(11) 2_575 ?
Te1 Ni1 3.1074(11) 2_675 ?
Te1 Na5 3.1780(13) 2_566 ?
Te1 Na5 3.2021(13) 2_666 ?
Te1 Na1 3.2138(10) 1_565 ?
Ni1 O1 2.0989(16) 2_575 ?
Ni1 O3 2.1121(16) 2_675 ?
Ni1 O4 2.1124(16) . ?
Ni1 O5 2.1194(17) . ?
Ni1 O5 2.1237(17) 2_575 ?
Ni1 O4 2.1321(17) 2_675 ?
Ni1 Te1 3.1017(11) 2_575 ?
Ni1 Te1 3.1074(11) 2_675 ?
Ni1 Na2 3.1714(13) 2_665 ?
Ni1 Na3 3.1994(13) 2_675 ?
Ni1 Na5 3.2227(19) 1_564 ?
O1 Ni1 2.0989(16) 2_575 ?
O1 Na1 2.2609(16) 1_565 ?
O1 Na5 2.3424(19) 2_566 ?
O1 Na3 2.4422(18) 1_465 ?
O1 Na2 2.4877(19) 1_465 ?
O2 Na2 2.2944(18) 1_565 ?
O2 Na5 2.3074(18) 2_666 ?
O2 Na3 2.3194(18) 1_465 ?
O2 Na5 2.3296(19) 1_565 ?
O2 Na4 2.7559(16) 1_565 ?
O3 Ni1 2.1121(16) 2_675 ?
O3 Na2 2.3012(18) . ?
O3 Na5 2.3956(18) 2_666 ?
O3 Na4 2.4343(17) . ?
O3 Na3 2.4564(19) . ?
O4 Ni1 2.1321(16) 2_675 ?
O4 Na1 2.3807(16) 1_565 ?
O4 Na2 2.3878(18) 1_565 ?
O4 Na2 2.4476(19) 2_675 ?
O5 Ni1 2.1237(17) 2_575 ?
O5 Na2 2.4296(19) . ?
O5 Na3 2.4679(19) 1_455 ?
O5 Na1 2.5142(16) . ?
O6 Na4 2.2384(16) . ?
O6 Na3 2.3029(18) 1_455 ?
O6 Na5 2.3057(18) 2_566 ?
O6 Na5 2.4191(18) 1_565 ?
O6 Na3 2.595(2) 2_666 ?
Na1 O1 2.2609(16) 2_575 ?
Na1 O1 2.2609(16) 1_545 ?
Na1 O4 2.3807(16) 1_545 ?
Na1 O4 2.3807(16) 2_575 ?
Na1 O5 2.5142(16) 2_565 ?
Na1 Na2 3.0509(13) 2_665 ?
Na1 Na2 3.0509(13) 1_455 ?
Na1 Na2 3.1218(13) . ?
Na1 Na2 3.1218(13) 2_565 ?
Na1 Na3 3.1537(19) 2_665 ?
Na1 Na3 3.1537(19) 1_455 ?
Na2 O2 2.2944(18) 1_545 ?
Na2 O4 2.3878(18) 1_545 ?
Na2 O4 2.4476(19) 2_675 ?
Na2 O1 2.4877(18) 1_645 ?
Na2 Na2 2.982(2) 2_665 ?
Na2 Na1 3.0509(13) 1_655 ?
Na2 Na3 3.0611(16) . ?
Na2 Ni1 3.1714(13) 2_665 ?
Na3 O6 2.3029(18) 1_655 ?
Na3 O2 2.3194(18) 1_645 ?
Na3 O1 2.4422(18) 1_645 ?
Na3 O5 2.4679(19) 1_655 ?
Na3 O6 2.595(2) 2_666 ?
Na3 Na4 3.0531(13) . ?
Na3 Na1 3.1537(19) 1_655 ?
Na3 Na5 3.1637(15) 2_656 ?
Na3 Ni1 3.1994(13) 2_675 ?
Na3 Na5 3.2201(15) 1_655 ?
Na4 O6 2.2384(16) 2_666 ?
Na4 O3 2.4343(17) 2_666 ?
Na4 O2 2.7559(16) 1_545 ?
Na4 O2 2.7559(16) 2_676 ?
Na4 Na3 3.0531(13) 2_666 ?
Na4 Na5 3.2055(12) 2_666 ?
Na4 Na5 3.2055(12) . ?
Na4 Te1 3.2343(10) 2_666 ?
Na5 O6 2.3057(18) 2_566 ?
Na5 O2 2.3074(18) 2_666 ?
Na5 O2 2.3296(19) 1_545 ?
Na5 O1 2.3424(19) 2_566 ?
Na5 O3 2.3956(18) 2_666 ?
Na5 O6 2.4191(18) 1_545 ?
Na5 Na5 3.0832(18) 2_656 ?
Na5 Na5 3.1466(18) 2_556 ?
Na5 Na3 3.1637(15) 2_656 ?
Na5 Te1 3.1780(13) 2_566 ?
Na5 Te1 3.2021(13) 2_666 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Te1 O6 92.87(7) . . ?
O2 Te1 O3 93.30(7) . . ?
O6 Te1 O3 91.09(7) . . ?
O2 Te1 O1 90.80(7) . . ?
O6 Te1 O1 92.86(7) . . ?
O3 Te1 O1 174.16(6) . . ?
O2 Te1 O5 173.28(6) . . ?
O6 Te1 O5 91.99(7) . . ?
O3 Te1 O5 91.24(7) . . ?
O1 Te1 O5 84.32(7) . . ?
O2 Te1 O4 90.42(7) . . ?
O6 Te1 O4 174.84(6) . . ?
O3 Te1 O4 84.75(7) . . ?
O1 Te1 O4 91.06(7) . . ?
O5 Te1 O4 85.07(7) . . ?
O2 Te1 Ni1 132.70(5) . . ?
O6 Te1 Ni1 134.43(5) . . ?
O3 Te1 Ni1 87.22(5) . . ?
O1 Te1 Ni1 86.94(5) . . ?
O5 Te1 Ni1 42.60(4) . . ?
O4 Te1 Ni1 42.47(5) . . ?
O2 Te1 Ni1 132.62(5) . 2_575 ?
O6 Te1 Ni1 90.22(5) . 2_575 ?
O3 Te1 Ni1 133.91(5) . 2_575 ?
O1 Te1 Ni1 41.83(5) . 2_575 ?
O5 Te1 Ni1 42.68(4) . 2_575 ?
O4 Te1 Ni1 90.47(5) . 2_575 ?
Ni1 Te1 Ni1 60.53(2) . 2_575 ?
O2 Te1 Ni1 89.53(5) . 2_675 ?
O6 Te1 Ni1 133.14(5) . 2_675 ?
O3 Te1 Ni1 42.06(5) . 2_675 ?
O1 Te1 Ni1 133.92(5) . 2_675 ?
O5 Te1 Ni1 90.53(5) . 2_675 ?
O4 Te1 Ni1 42.86(5) . 2_675 ?
Ni1 Te1 Ni1 60.50(2) . 2_675 ?
Ni1 Te1 Ni1 121.03(3) 2_575 2_675 ?
O2 Te1 Na5 87.80(5) . 2_566 ?
O6 Te1 Na5 46.01(5) . 2_566 ?
O3 Te1 Na5 137.04(5) . 2_566 ?
O1 Te1 Na5 47.25(5) . 2_566 ?
O5 Te1 Na5 92.24(5) . 2_566 ?
O4 Te1 Na5 138.21(5) . 2_566 ?
Ni1 Te1 Na5 122.26(3) . 2_566 ?
Ni1 Te1 Na5 61.74(4) 2_575 2_566 ?
Ni1 Te1 Na5 177.119(14) 2_675 2_566 ?
O2 Te1 Na5 45.41(5) . 2_666 ?
O6 Te1 Na5 88.30(6) . 2_666 ?
O3 Te1 Na5 48.24(5) . 2_666 ?
O1 Te1 Na5 136.16(5) . 2_666 ?
O5 Te1 Na5 139.47(5) . 2_666 ?
O4 Te1 Na5 91.19(6) . 2_666 ?
Ni1 Te1 Na5 121.90(3) . 2_666 ?
Ni1 Te1 Na5 177.438(13) 2_575 2_666 ?
Ni1 Te1 Na5 61.41(4) 2_675 2_666 ?
Na5 Te1 Na5 115.81(4) 2_566 2_666 ?
O2 Te1 Na1 85.06(6) . 1_565 ?
O6 Te1 Na1 136.64(5) . 1_565 ?
O3 Te1 Na1 132.27(5) . 1_565 ?
O1 Te1 Na1 44.00(4) . 1_565 ?
O5 Te1 Na1 88.23(5) . 1_565 ?
O4 Te1 Na1 47.64(5) . 1_565 ?
Ni1 Te1 Na1 61.45(2) . 1_565 ?
Ni1 Te1 Na1 61.82(2) 2_575 1_565 ?
Ni1 Te1 Na1 90.21(3) 2_675 1_565 ?
Na5 Te1 Na1 90.64(3) 2_566 1_565 ?
Na5 Te1 Na1 118.17(3) 2_666 1_565 ?
O1 Ni1 O3 94.55(7) 2_575 2_675 ?
O1 Ni1 O4 171.45(6) 2_575 . ?
O3 Ni1 O4 93.24(7) 2_675 . ?
O1 Ni1 O5 93.50(7) 2_575 . ?
O3 Ni1 O5 171.14(6) 2_675 . ?
O4 Ni1 O5 78.97(7) . . ?
O1 Ni1 O5 77.47(6) 2_575 2_575 ?
O3 Ni1 O5 100.26(6) 2_675 2_575 ?
O4 Ni1 O5 97.69(6) . 2_575 ?
O5 Ni1 O5 85.12(6) . 2_575 ?
O1 Ni1 O4 99.99(6) 2_575 2_675 ?
O3 Ni1 O4 77.70(6) 2_675 2_675 ?
O4 Ni1 O4 85.09(6) . 2_675 ?
O5 Ni1 O4 97.24(6) . 2_675 ?
O5 Ni1 O4 176.67(5) 2_575 2_675 ?
O1 Ni1 Te1 132.63(4) 2_575 . ?
O3 Ni1 Te1 132.82(5) 2_675 . ?
O4 Ni1 Te1 39.72(4) . . ?
O5 Ni1 Te1 39.26(4) . . ?
O5 Ni1 Te1 91.82(4) 2_575 . ?
O4 Ni1 Te1 91.49(4) 2_675 . ?
O1 Ni1 Te1 38.40(4) 2_575 2_575 ?
O3 Ni1 Te1 96.77(5) 2_675 2_575 ?
O4 Ni1 Te1 136.85(4) . 2_575 ?
O5 Ni1 Te1 91.85(5) . 2_575 ?
O5 Ni1 Te1 39.23(4) 2_575 2_575 ?
O4 Ni1 Te1 138.04(4) 2_675 2_575 ?
Te1 Ni1 Te1 119.47(2) . 2_575 ?
O1 Ni1 Te1 96.64(5) 2_575 2_675 ?
O3 Ni1 Te1 38.22(4) 2_675 2_675 ?
O4 Ni1 Te1 91.65(5) . 2_675 ?
O5 Ni1 Te1 136.79(4) . 2_675 ?
O5 Ni1 Te1 138.09(4) 2_575 2_675 ?
O4 Ni1 Te1 39.63(4) 2_675 2_675 ?
Te1 Ni1 Te1 119.50(2) . 2_675 ?
Te1 Ni1 Te1 121.03(3) 2_575 2_675 ?
O1 Ni1 Na2 51.57(5) 2_575 2_665 ?
O3 Ni1 Na2 88.99(5) 2_675 2_665 ?
O4 Ni1 Na2 132.18(5) . 2_665 ?
O5 Ni1 Na2 93.10(5) . 2_665 ?
O5 Ni1 Na2 128.86(5) 2_575 2_665 ?
O4 Ni1 Na2 48.83(4) 2_675 2_665 ?
Te1 Ni1 Na2 117.87(2) . 2_665 ?
Te1 Ni1 Na2 89.97(3) 2_575 2_665 ?
Te1 Ni1 Na2 62.52(2) 2_675 2_665 ?
O1 Ni1 Na3 88.39(5) 2_575 2_675 ?
O3 Ni1 Na3 50.13(5) 2_675 2_675 ?
O4 Ni1 Na3 93.94(6) . 2_675 ?
O5 Ni1 Na3 133.94(5) . 2_675 ?
O5 Ni1 Na3 50.43(5) 2_575 2_675 ?
O4 Ni1 Na3 127.74(5) 2_675 2_675 ?
Te1 Ni1 Na3 119.78(3) . 2_675 ?
Te1 Ni1 Na3 62.72(3) 2_575 2_675 ?
Te1 Ni1 Na3 88.35(3) 2_675 2_675 ?
Na2 Ni1 Na3 122.35(4) 2_665 2_675 ?
O1 Ni1 Na5 46.54(4) 2_575 1_564 ?
O3 Ni1 Na5 48.01(5) 2_675 1_564 ?
O4 Ni1 Na5 141.15(5) . 1_564 ?
O5 Ni1 Na5 139.88(5) . 1_564 ?
O5 Ni1 Na5 88.42(4) 2_575 1_564 ?
O4 Ni1 Na5 88.26(4) 2_675 1_564 ?
Te1 Ni1 Na5 179.048(17) . 1_564 ?
Te1 Ni1 Na5 60.29(2) 2_575 1_564 ?
Te1 Ni1 Na5 60.74(2) 2_675 1_564 ?
Na2 Ni1 Na5 61.33(2) 2_665 1_564 ?
Na3 Ni1 Na5 61.04(3) 2_675 1_564 ?
Te1 O1 Ni1 99.77(7) . 2_575 ?
Te1 O1 Na1 99.08(6) . 1_565 ?
Ni1 O1 Na1 96.15(7) 2_575 1_565 ?
Te1 O1 Na5 94.95(7) . 2_566 ?
Ni1 O1 Na5 92.88(7) 2_575 2_566 ?
Na1 O1 Na5 161.75(7) 1_565 2_566 ?
Te1 O1 Na3 96.43(6) . 1_465 ?
Ni1 O1 Na3 163.53(8) 2_575 1_465 ?
Na1 O1 Na3 84.13(6) 1_565 1_465 ?
Na5 O1 Na3 82.76(6) 2_566 1_465 ?
Te1 O1 Na2 173.16(8) . 1_465 ?
Ni1 O1 Na2 87.06(6) 2_575 1_465 ?
Na1 O1 Na2 79.80(5) 1_565 1_465 ?
Na5 O1 Na2 84.88(6) 2_566 1_465 ?
Na3 O1 Na2 76.76(5) 1_465 1_465 ?
Te1 O2 Na2 101.66(7) . 1_565 ?
Te1 O2 Na5 98.77(7) . 2_666 ?
Na2 O2 Na5 90.26(6) 1_565 2_666 ?
Te1 O2 Na3 102.35(7) . 1_465 ?
Na2 O2 Na3 90.83(6) 1_565 1_465 ?
Na5 O2 Na3 158.18(7) 2_666 1_465 ?
Te1 O2 Na5 99.78(7) . 1_565 ?
Na2 O2 Na5 158.32(8) 1_565 1_565 ?
Na5 O2 Na5 83.35(6) 2_666 1_565 ?
Na3 O2 Na5 87.68(6) 1_465 1_565 ?
Te1 O2 Na4 176.86(8) . 1_565 ?
Na2 O2 Na4 80.82(6) 1_565 1_565 ?
Na5 O2 Na4 79.22(5) 2_666 1_565 ?
Na3 O2 Na4 79.44(5) 1_465 1_565 ?
Na5 O2 Na4 77.65(6) 1_565 1_565 ?
Te1 O3 Ni1 99.71(7) . 2_675 ?
Te1 O3 Na2 100.20(7) . . ?
Ni1 O3 Na2 94.01(7) 2_675 . ?
Te1 O3 Na5 94.35(6) . 2_666 ?
Ni1 O3 Na5 91.05(7) 2_675 2_666 ?
Na2 O3 Na5 163.54(8) . 2_666 ?
Te1 O3 Na4 94.41(6) . . ?
Ni1 O3 Na4 165.12(8) 2_675 . ?
Na2 O3 Na4 88.06(6) . . ?
Na5 O3 Na4 83.16(6) 2_666 . ?
Te1 O3 Na3 171.66(8) . . ?
Ni1 O3 Na3 88.57(6) 2_675 . ?
Na2 O3 Na3 80.02(6) . . ?
Na5 O3 Na3 84.46(6) 2_666 . ?
Na4 O3 Na3 77.26(5) . . ?
Te1 O4 Ni1 97.82(7) . . ?
Te1 O4 Ni1 97.51(7) . 2_675 ?
Ni1 O4 Ni1 94.91(6) . 2_675 ?
Te1 O4 Na1 94.00(6) . 1_565 ?
Ni1 O4 Na1 91.62(6) . 1_565 ?
Ni1 O4 Na1 165.86(8) 2_675 1_565 ?
Te1 O4 Na2 95.53(7) . 1_565 ?
Ni1 O4 Na2 165.50(8) . 1_565 ?
Ni1 O4 Na2 88.94(6) 2_675 1_565 ?
Na1 O4 Na2 81.79(6) 1_565 1_565 ?
Te1 O4 Na2 169.33(8) . 2_675 ?
Ni1 O4 Na2 89.91(7) . 2_675 ?
Ni1 O4 Na2 89.10(6) 2_675 2_675 ?
Na1 O4 Na2 78.36(5) 1_565 2_675 ?
Na2 O4 Na2 76.14(6) 1_565 2_675 ?
Te1 O5 Ni1 98.14(7) . . ?
Te1 O5 Ni1 98.10(6) . 2_575 ?
Ni1 O5 Ni1 94.88(6) . 2_575 ?
Te1 O5 Na2 95.14(7) . . ?
Ni1 O5 Na2 89.87(6) . . ?
Ni1 O5 Na2 165.15(8) 2_575 . ?
Te1 O5 Na3 94.37(7) . 1_455 ?
Ni1 O5 Na3 166.62(7) . 1_455 ?
Ni1 O5 Na3 88.01(6) 2_575 1_455 ?
Na2 O5 Na3 84.28(6) . 1_455 ?
Te1 O5 Na1 170.70(8) . . ?
Ni1 O5 Na1 88.50(6) . . ?
Ni1 O5 Na1 87.76(6) 2_575 . ?
Na2 O5 Na1 78.29(5) . . ?
Na3 O5 Na1 78.54(6) 1_455 . ?
Te1 O6 Na4 102.20(7) . . ?
Te1 O6 Na3 101.91(7) . 1_455 ?
Na4 O6 Na3 91.77(6) . 1_455 ?
Te1 O6 Na5 97.44(7) . 2_566 ?
Na4 O6 Na5 159.43(7) . 2_566 ?
Na3 O6 Na5 90.09(6) 1_455 2_566 ?
Te1 O6 Na5 96.39(7) . 1_565 ?
Na4 O6 Na5 88.30(6) . 1_565 ?
Na3 O6 Na5 161.25(7) 1_455 1_565 ?
Na5 O6 Na5 83.48(6) 2_566 1_565 ?
Te1 O6 Na3 174.53(8) . 2_666 ?
Na4 O6 Na3 77.95(5) . 2_666 ?
Na3 O6 Na3 83.54(6) 1_455 2_666 ?
Na5 O6 Na3 81.92(6) 2_566 2_666 ?
Na5 O6 Na3 78.15(6) 1_565 2_666 ?
O1 Na1 O1 180.00(6) 2_575 1_545 ?
O1 Na1 O4 105.16(6) 2_575 1_545 ?
O1 Na1 O4 74.84(6) 1_545 1_545 ?
O1 Na1 O4 74.84(6) 2_575 2_575 ?
O1 Na1 O4 105.16(6) 1_545 2_575 ?
O4 Na1 O4 180.00(5) 1_545 2_575 ?
O1 Na1 O5 79.90(6) 2_575 . ?
O1 Na1 O5 100.10(6) 1_545 . ?
O4 Na1 O5 98.72(5) 1_545 . ?
O4 Na1 O5 81.28(5) 2_575 . ?
O1 Na1 O5 100.10(6) 2_575 2_565 ?
O1 Na1 O5 79.90(6) 1_545 2_565 ?
O4 Na1 O5 81.28(5) 1_545 2_565 ?
O4 Na1 O5 98.72(5) 2_575 2_565 ?
O5 Na1 O5 180.00(5) . 2_565 ?
O1 Na1 Na2 53.37(4) 2_575 2_665 ?
O1 Na1 Na2 126.63(4) 1_545 2_665 ?
O4 Na1 Na2 51.79(4) 1_545 2_665 ?
O4 Na1 Na2 128.21(4) 2_575 2_665 ?
O5 Na1 Na2 88.69(4) . 2_665 ?
O5 Na1 Na2 91.31(4) 2_565 2_665 ?
O1 Na1 Na2 126.63(4) 2_575 1_455 ?
O1 Na1 Na2 53.37(4) 1_545 1_455 ?
O4 Na1 Na2 128.21(4) 1_545 1_455 ?
O4 Na1 Na2 51.79(4) 2_575 1_455 ?
O5 Na1 Na2 91.31(4) . 1_455 ?
O5 Na1 Na2 88.69(4) 2_565 1_455 ?
Na2 Na1 Na2 180.00(3) 2_665 1_455 ?
O1 Na1 Na2 91.03(5) 2_575 . ?
O1 Na1 Na2 88.97(5) 1_545 . ?
O4 Na1 Na2 49.20(4) 1_545 . ?
O4 Na1 Na2 130.80(4) 2_575 . ?
O5 Na1 Na2 49.65(4) . . ?
O5 Na1 Na2 130.35(4) 2_565 . ?
Na2 Na1 Na2 57.76(4) 2_665 . ?
Na2 Na1 Na2 122.24(4) 1_455 . ?
O1 Na1 Na2 88.97(5) 2_575 2_565 ?
O1 Na1 Na2 91.03(5) 1_545 2_565 ?
O4 Na1 Na2 130.80(4) 1_545 2_565 ?
O4 Na1 Na2 49.20(4) 2_575 2_565 ?
O5 Na1 Na2 130.35(4) . 2_565 ?
O5 Na1 Na2 49.65(4) 2_565 2_565 ?
Na2 Na1 Na2 122.24(4) 2_665 2_565 ?
Na2 Na1 Na2 57.76(4) 1_455 2_565 ?
Na2 Na1 Na2 180.00(3) . 2_565 ?
O1 Na1 Na3 50.38(5) 2_575 2_665 ?
O1 Na1 Na3 129.62(5) 1_545 2_665 ?
O4 Na1 Na3 90.05(4) 1_545 2_665 ?
O4 Na1 Na3 89.95(4) 2_575 2_665 ?
O5 Na1 Na3 129.92(4) . 2_665 ?
O5 Na1 Na3 50.08(4) 2_565 2_665 ?
Na2 Na1 Na3 59.09(3) 2_665 2_665 ?
Na2 Na1 Na3 120.91(3) 1_455 2_665 ?
Na2 Na1 Na3 116.85(3) . 2_665 ?
Na2 Na1 Na3 63.15(3) 2_565 2_665 ?
O1 Na1 Na3 129.62(5) 2_575 1_455 ?
O1 Na1 Na3 50.38(5) 1_545 1_455 ?
O4 Na1 Na3 89.95(4) 1_545 1_455 ?
O4 Na1 Na3 90.05(4) 2_575 1_455 ?
O5 Na1 Na3 50.08(4) . 1_455 ?
O5 Na1 Na3 129.92(4) 2_565 1_455 ?
Na2 Na1 Na3 120.91(3) 2_665 1_455 ?
Na2 Na1 Na3 59.09(3) 1_455 1_455 ?
Na2 Na1 Na3 63.15(3) . 1_455 ?
Na2 Na1 Na3 116.85(3) 2_565 1_455 ?
Na3 Na1 Na3 180.00(3) 2_665 1_455 ?
O2 Na2 O3 102.56(7) 1_545 . ?
O2 Na2 O4 72.37(6) 1_545 1_545 ?
O3 Na2 O4 171.99(6) . 1_545 ?
O2 Na2 O5 93.17(6) 1_545 . ?
O3 Na2 O5 72.83(6) . . ?
O4 Na2 O5 100.93(6) 1_545 . ?
O2 Na2 O4 173.03(6) 1_545 2_675 ?
O3 Na2 O4 80.51(6) . 2_675 ?
O4 Na2 O4 103.86(6) 1_545 2_675 ?
O5 Na2 O4 81.70(6) . 2_675 ?
O2 Na2 O1 88.77(6) 1_545 1_645 ?
O3 Na2 O1 103.03(6) . 1_645 ?
O4 Na2 O1 83.30(6) 1_545 1_645 ?
O5 Na2 O1 175.72(6) . 1_645 ?
O4 Na2 O1 96.67(6) 2_675 1_645 ?
O2 Na2 Na2 124.91(6) 1_545 2_665 ?
O3 Na2 Na2 131.11(6) . 2_665 ?
O4 Na2 Na2 52.83(4) 1_545 2_665 ?
O5 Na2 Na2 91.90(5) . 2_665 ?
O4 Na2 Na2 51.02(5) 2_675 2_665 ?
O1 Na2 Na2 90.11(5) 1_645 2_665 ?
O2 Na2 Na1 135.39(5) 1_545 1_655 ?
O3 Na2 Na1 93.30(5) . 1_655 ?
O4 Na2 Na1 94.63(5) 1_545 1_655 ?
O5 Na2 Na1 131.43(5) . 1_655 ?
O4 Na2 Na1 49.84(4) 2_675 1_655 ?
O1 Na2 Na1 46.83(4) 1_645 1_655 ?
Na2 Na2 Na1 62.31(4) 2_665 1_655 ?
O2 Na2 Na3 95.80(6) 1_545 . ?
O3 Na2 Na3 52.21(4) . . ?
O4 Na2 Na3 133.48(5) 1_545 . ?
O5 Na2 Na3 124.98(5) . . ?
O4 Na2 Na3 91.01(5) 2_675 . ?
O1 Na2 Na3 50.95(5) 1_645 . ?
Na2 Na2 Na3 124.43(5) 2_665 . ?
Na1 Na2 Na3 62.13(4) 1_655 . ?
O2 Na2 Na1 81.43(5) 1_545 . ?
O3 Na2 Na1 124.87(5) . . ?
O4 Na2 Na1 49.01(4) 1_545 . ?
O5 Na2 Na1 52.06(4) . . ?
O4 Na2 Na1 91.68(5) 2_675 . ?
O1 Na2 Na1 132.10(5) 1_645 . ?
Na2 Na2 Na1 59.92(3) 2_665 . ?
Na1 Na2 Na1 122.24(4) 1_655 . ?
Na3 Na2 Na1 175.56(4) . . ?
O2 Na2 Ni1 81.44(5) 1_545 2_665 ?
O3 Na2 Ni1 144.39(5) . 2_665 ?
O4 Na2 Ni1 42.23(4) 1_545 2_665 ?
O5 Na2 Ni1 142.74(5) . 2_665 ?
O4 Na2 Ni1 99.77(5) 2_675 2_665 ?
O1 Na2 Ni1 41.37(4) 1_645 2_665 ?
Na2 Na2 Ni1 63.03(3) 2_665 2_665 ?
Na1 Na2 Ni1 62.84(2) 1_655 2_665 ?
Na3 Na2 Ni1 92.28(3) . 2_665 ?
Na1 Na2 Ni1 90.73(3) . 2_665 ?
O2 Na2 Ni1 132.57(5) 1_545 . ?
O3 Na2 Ni1 78.94(6) . . ?
O4 Na2 Ni1 99.77(6) 1_545 . ?
O5 Na2 Ni1 41.15(4) . . ?
O4 Na2 Ni1 41.45(4) 2_675 . ?
O1 Na2 Ni1 137.79(5) 1_645 . ?
Na2 Na2 Ni1 61.36(4) 2_665 . ?
Na1 Na2 Ni1 91.10(3) 1_655 . ?
Na3 Na2 Ni1 118.97(4) . . ?
Na1 Na2 Ni1 61.53(3) . . ?
Ni1 Na2 Ni1 124.39(4) 2_665 . ?
O6 Na3 O2 98.06(7) 1_655 1_645 ?
O6 Na3 O1 163.63(6) 1_655 1_645 ?
O2 Na3 O1 70.28(6) 1_645 1_645 ?
O6 Na3 O3 90.05(6) 1_655 . ?
O2 Na3 O3 168.07(7) 1_645 . ?
O1 Na3 O3 99.92(6) 1_645 . ?
O6 Na3 O5 71.73(7) 1_655 1_655 ?
O2 Na3 O5 91.57(6) 1_645 1_655 ?
O1 Na3 O5 96.53(6) 1_645 1_655 ?
O3 Na3 O5 82.63(6) . 1_655 ?
O6 Na3 O6 96.46(6) 1_655 2_666 ?
O2 Na3 O6 90.99(6) 1_645 2_666 ?
O1 Na3 O6 95.21(6) 1_645 2_666 ?
O3 Na3 O6 96.81(6) . 2_666 ?
O5 Na3 O6 168.17(6) 1_655 2_666 ?
O6 Na3 Na4 96.80(5) 1_655 . ?
O2 Na3 Na4 135.62(5) 1_645 . ?
O1 Na3 Na4 99.57(5) 1_645 . ?
O3 Na3 Na4 51.05(4) . . ?
O5 Na3 Na4 132.81(5) 1_655 . ?
O6 Na3 Na4 45.81(4) 2_666 . ?
O6 Na3 Na2 137.04(5) 1_655 . ?
O2 Na3 Na2 122.49(5) 1_645 . ?
O1 Na3 Na2 52.29(4) 1_645 . ?
O3 Na3 Na2 47.77(5) . . ?
O5 Na3 Na2 91.97(5) 1_655 . ?
O6 Na3 Na2 96.39(6) 2_666 . ?
Na4 Na3 Na2 65.17(4) . . ?
O6 Na3 Na1 122.86(5) 1_655 1_655 ?
O2 Na3 Na1 80.35(5) 1_645 1_655 ?
O1 Na3 Na1 45.49(4) 1_645 1_655 ?
O3 Na3 Na1 87.90(5) . 1_655 ?
O5 Na3 Na1 51.38(4) 1_655 1_655 ?
O6 Na3 Na1 140.45(5) 2_666 1_655 ?
Na4 Na3 Na1 123.92(4) . 1_655 ?
Na2 Na3 Na1 58.78(3) . 1_655 ?
O6 Na3 Na5 144.73(5) 1_655 2_656 ?
O2 Na3 Na5 81.55(5) 1_645 2_656 ?
O1 Na3 Na5 47.26(4) 1_645 2_656 ?
O3 Na3 Na5 96.88(5) . 2_656 ?
O5 Na3 Na5 143.39(5) 1_655 2_656 ?
O6 Na3 Na5 48.45(4) 2_666 2_656 ?
Na4 Na3 Na5 62.94(3) . 2_656 ?
Na2 Na3 Na5 63.16(3) . 2_656 ?
Na1 Na3 Na5 92.02(3) 1_655 2_656 ?
O6 Na3 Ni1 81.30(5) 1_655 2_675 ?
O2 Na3 Ni1 131.25(5) 1_645 2_675 ?
O1 Na3 Ni1 97.60(6) 1_645 2_675 ?
O3 Na3 Ni1 41.30(4) . 2_675 ?
O5 Na3 Ni1 41.56(4) 1_655 2_675 ?
O6 Na3 Ni1 137.71(5) 2_666 2_675 ?
Na4 Na3 Ni1 92.25(3) . 2_675 ?
Na2 Na3 Ni1 62.09(3) . 2_675 ?
Na1 Na3 Ni1 61.05(3) 1_655 2_675 ?
Na5 Na3 Ni1 125.22(4) 2_656 2_675 ?
O6 Na3 Na5 95.27(6) 1_655 1_655 ?
O2 Na3 Na5 46.29(5) 1_645 1_655 ?
O1 Na3 Na5 84.91(5) 1_645 1_655 ?
O3 Na3 Na5 141.92(5) . 1_655 ?
O5 Na3 Na5 134.72(5) 1_655 1_655 ?
O6 Na3 Na5 45.15(4) 2_666 1_655 ?
Na4 Na3 Na5 90.88(4) . 1_655 ?
Na2 Na3 Na5 122.13(4) . 1_655 ?
Na1 Na3 Na5 119.36(4) 1_655 1_655 ?
Na5 Na3 Na5 59.06(4) 2_656 1_655 ?
Ni1 Na3 Na5 175.61(4) 2_675 1_655 ?
O6 Na4 O6 180.00(8) . 2_666 ?
O6 Na4 O3 72.12(6) . . ?
O6 Na4 O3 107.88(6) 2_666 . ?
O6 Na4 O3 107.88(6) . 2_666 ?
O6 Na4 O3 72.12(6) 2_666 2_666 ?
O3 Na4 O3 180.0 . 2_666 ?
O6 Na4 O2 88.03(6) . 1_545 ?
O6 Na4 O2 91.97(6) 2_666 1_545 ?
O3 Na4 O2 87.16(6) . 1_545 ?
O3 Na4 O2 92.84(6) 2_666 1_545 ?
O6 Na4 O2 91.97(6) . 2_676 ?
O6 Na4 O2 88.03(6) 2_666 2_676 ?
O3 Na4 O2 92.84(6) . 2_676 ?
O3 Na4 O2 87.16(6) 2_666 2_676 ?
O2 Na4 O2 180.00(5) 1_545 2_676 ?
O6 Na4 Na3 123.76(5) . . ?
O6 Na4 Na3 56.24(5) 2_666 . ?
O3 Na4 Na3 51.70(4) . . ?
O3 Na4 Na3 128.30(4) 2_666 . ?
O2 Na4 Na3 87.06(4) 1_545 . ?
O2 Na4 Na3 92.94(4) 2_676 . ?
O6 Na4 Na3 56.24(5) . 2_666 ?
O6 Na4 Na3 123.76(5) 2_666 2_666 ?
O3 Na4 Na3 128.30(4) . 2_666 ?
O3 Na4 Na3 51.70(4) 2_666 2_666 ?
O2 Na4 Na3 92.94(4) 1_545 2_666 ?
O2 Na4 Na3 87.06(4) 2_676 2_666 ?
Na3 Na4 Na3 180.0 . 2_666 ?
O6 Na4 Na5 82.99(5) . 2_666 ?
O6 Na4 Na5 97.01(5) 2_666 2_666 ?
O3 Na4 Na5 47.90(4) . 2_666 ?
O3 Na4 Na5 132.10(4) 2_666 2_666 ?
O2 Na4 Na5 134.77(4) 1_545 2_666 ?
O2 Na4 Na5 45.23(4) 2_676 2_666 ?
Na3 Na4 Na5 62.76(3) . 2_666 ?
Na3 Na4 Na5 117.24(3) 2_666 2_666 ?
O6 Na4 Na5 97.01(5) . . ?
O6 Na4 Na5 82.99(5) 2_666 . ?
O3 Na4 Na5 132.10(4) . . ?
O3 Na4 Na5 47.90(4) 2_666 . ?
O2 Na4 Na5 45.23(4) 1_545 . ?
O2 Na4 Na5 134.77(4) 2_676 . ?
Na3 Na4 Na5 117.24(3) . . ?
Na3 Na4 Na5 62.76(3) 2_666 . ?
Na5 Na4 Na5 180.0 2_666 . ?
O6 Na4 Te1 35.23(4) . . ?
O6 Na4 Te1 144.77(4) 2_666 . ?
O3 Na4 Te1 36.97(4) . . ?
O3 Na4 Te1 143.03(4) 2_666 . ?
O2 Na4 Te1 88.81(5) 1_545 . ?
O2 Na4 Te1 91.19(5) 2_676 . ?
Na3 Na4 Te1 88.66(3) . . ?
Na3 Na4 Te1 91.34(3) 2_666 . ?
Na5 Na4 Te1 59.63(3) 2_666 . ?
Na5 Na4 Te1 120.37(3) . . ?
O6 Na4 Te1 144.77(4) . 2_666 ?
O6 Na4 Te1 35.23(4) 2_666 2_666 ?
O3 Na4 Te1 143.03(4) . 2_666 ?
O3 Na4 Te1 36.97(4) 2_666 2_666 ?
O2 Na4 Te1 91.19(5) 1_545 2_666 ?
O2 Na4 Te1 88.81(5) 2_676 2_666 ?
Na3 Na4 Te1 91.34(3) . 2_666 ?
Na3 Na4 Te1 88.66(3) 2_666 2_666 ?
Na5 Na4 Te1 120.37(3) 2_666 2_666 ?
Na5 Na4 Te1 59.63(3) . 2_666 ?
Te1 Na4 Te1 180.0 . 2_666 ?
O6 Na5 O2 160.80(6) 2_566 2_666 ?
O6 Na5 O2 98.46(6) 2_566 1_545 ?
O2 Na5 O2 96.65(6) 2_666 1_545 ?
O6 Na5 O1 74.07(6) 2_566 2_566 ?
O2 Na5 O1 92.10(6) 2_666 2_566 ?
O2 Na5 O1 169.98(7) 1_545 2_566 ?
O6 Na5 O3 91.51(6) 2_566 2_666 ?
O2 Na5 O3 72.98(6) 2_666 2_666 ?
O2 Na5 O3 105.70(7) 1_545 2_666 ?
O1 Na5 O3 81.52(7) 2_566 2_666 ?
O6 Na5 O6 96.52(6) 2_566 1_545 ?
O2 Na5 O6 99.56(6) 2_666 1_545 ?
O2 Na5 O6 70.96(6) 1_545 1_545 ?
O1 Na5 O6 102.82(7) 2_566 1_545 ?
O3 Na5 O6 171.66(6) 2_666 1_545 ?
O6 Na5 Na5 144.88(6) 2_566 2_656 ?
O2 Na5 Na5 48.63(5) 2_666 2_656 ?
O2 Na5 Na5 48.02(4) 1_545 2_656 ?
O1 Na5 Na5 140.49(6) 2_566 2_656 ?
O3 Na5 Na5 89.16(5) 2_666 2_656 ?
O6 Na5 Na5 82.98(5) 1_545 2_656 ?
O6 Na5 Na5 49.80(5) 2_566 2_556 ?
O2 Na5 Na5 145.06(6) 2_666 2_556 ?
O2 Na5 Na5 81.78(6) 1_545 2_556 ?
O1 Na5 Na5 88.25(6) 2_566 2_556 ?
O3 Na5 Na5 141.26(5) 2_666 2_556 ?
O6 Na5 Na5 46.72(4) 1_545 2_556 ?
Na5 Na5 Na5 120.36(6) 2_656 2_556 ?
O6 Na5 Na3 88.36(5) 2_566 2_656 ?
O2 Na5 Na3 92.83(5) 2_666 2_656 ?
O2 Na5 Na3 124.37(5) 1_545 2_656 ?
O1 Na5 Na3 49.98(4) 2_566 2_656 ?
O3 Na5 Na3 129.39(5) 2_666 2_656 ?
O6 Na5 Na3 53.41(5) 1_545 2_656 ?
Na5 Na5 Na3 117.61(4) 2_656 2_656 ?
Na5 Na5 Na3 61.37(3) 2_556 2_656 ?
O6 Na5 Te1 36.56(4) 2_566 2_566 ?
O2 Na5 Te1 129.48(5) 2_666 2_566 ?
O2 Na5 Te1 133.85(5) 1_545 2_566 ?
O1 Na5 Te1 37.80(4) 2_566 2_566 ?
O3 Na5 Te1 89.20(5) 2_666 2_566 ?
O6 Na5 Te1 98.58(5) 1_545 2_566 ?
Na5 Na5 Te1 177.87(4) 2_656 2_566 ?
Na5 Na5 Te1 61.71(4) 2_556 2_566 ?
Na3 Na5 Te1 62.61(3) 2_656 2_566 ?
O6 Na5 Te1 128.65(5) 2_566 2_666 ?
O2 Na5 Te1 35.82(4) 2_666 2_666 ?
O2 Na5 Te1 100.61(5) 1_545 2_666 ?
O1 Na5 Te1 89.35(5) 2_566 2_666 ?
O3 Na5 Te1 37.40(4) 2_666 2_666 ?
O6 Na5 Te1 134.76(5) 1_545 2_666 ?
Na5 Na5 Te1 62.11(4) 2_656 2_666 ?
Na5 Na5 Te1 177.48(4) 2_556 2_666 ?
Na3 Na5 Te1 117.42(3) 2_656 2_666 ?
Te1 Na5 Te1 115.81(4) 2_566 2_666 ?
O6 Na5 Na4 92.71(5) 2_566 . ?
O2 Na5 Na4 85.61(5) 2_666 . ?
O2 Na5 Na4 57.12(4) 1_545 . ?
O1 Na5 Na4 128.79(5) 2_566 . ?
O3 Na5 Na4 48.94(4) 2_666 . ?
O6 Na5 Na4 128.06(5) 1_545 . ?
Na5 Na5 Na4 62.13(3) 2_656 . ?
Na5 Na5 Na4 120.56(4) 2_556 . ?
Na3 Na5 Na4 178.01(3) 2_656 . ?
Te1 Na5 Na4 117.57(3) 2_566 . ?
Te1 Na5 Na4 60.63(2) 2_666 . ?

_diffrn_measured_fraction_theta_max 0.977
_diffrn_reflns_theta_full        27.50
_diffrn_measured_fraction_theta_full 0.977
_refine_diff_density_max         0.443
_refine_diff_density_min         -0.737
_refine_diff_density_rms         0.100
